Post-Cracking Properties of Concrete Reinforced with Polypropylene Fibers through the Barcelona Test

The Barcelona method was developed as an alternative to other tests for assessing the post-cracking behavior of fiber-reinforced concrete, with the main advantage being that it uses significantly smaller specimens compared to other methods. For this reason, it can provide a solution for characterizing concrete in hard-to-reach constructions such as roads and tunnels. On the other hand, polypropylene (PP) fibers have gained increased attention in recent years within the scientific community due to their high tensile strength and cost-effectiveness. This research aimed to understand the influence of PP fiber volume, slenderness (l/d), and reinforcement index on post-cracking properties of concrete, including toughness and residual strength (f_res), using the Barcelona method. Three fiber volumes, 0.4%, 0.8%, and 1.2%, and three slenderness ratios, 46.5, 58.1, and 69.8, were employed in normal-strength concrete. In addition to the reference mixture without fibers, 10 mixtures were prepared with 10 specimens each, resulting in a total of 100 specimens. Pearson’s hypothesis test was employed to determine the existence of correlations between variables, followed by scatter plots to generate predictive equations between post-cracking properties and fiber attributes. The results indicated no direct correlation between fiber slenderness and post-cracking properties. Regarding fiber volume, there was a correlation with residual strength but not with toughness. However, the combined effect of volume and slenderness, the reinforcement index, correlates with the post-cracking properties of concrete. Finally, four predictive equations for toughness and residual strength were derived based on the reinforcement index. These equations can prove valuable for designing structures made of polypropylene fiber-reinforced concrete.


Introduction
In the realm of contemporary construction, plain concrete stands out as an essential material due to its simplicity and versatility, being used in various structures and projects.However, the increasing demands for structural strength and durability have revealed plain concrete's limitations under intense stress and load, leading to the emergence of fiberreinforced concrete (FRC).Compared with plain concrete, FRC is known for its enhanced residual strengths and toughness [1,2].The FRC is widely applied in constructing subway tunnels, industrial floors, rail bases, machine foundations, and underground mining [3].The energy absorption capacity, or toughness, is an important characteristic of structures subjected to seismic, fatigue, impact, and blast loads [4].The toughness of a specimen is equal to the area under its load-deflection curve up to a certain displacement [5].Its magnitude depends directly on the geometry of the test specimen and the type of fibers [6].
The most used fibers are steel and polypropylene fibers.PP fibers are synthetic fibers made from isotactic polypropylene polymerized with propylene [7].This type of fiber has a high melting point (165 • C) and good corrosion resistance.Due to their hydrophobicity, polypropylene fibers can be evenly distributed in concrete [8].In addition, they have a Polymers 2023, 15, 3718 2 of 17 greater effect on shrinkage reduction and decrease the spalling effect in high-strength FRC subjected to high temperatures [9].Del Savio et al. (2022) [10] found that PP fibers with lengths of 50 and 60 mm increase 34% and 35%, respectively, in the tensile strength when the dosage is at 1.20%.Also, PP fibers with lengths of 60 mm show an increase of 3.80, 8.46, and 12.09% when the dosage is 0.4, 0.8, and 1.2%, respectively, in the modulus of rupture.
On the other hand, since the decade of 2010, the Barcelona method has been developed to evaluate toughness, and the test configuration consists of double punching a cylinder with a slenderness equal to unity.This method is more economical than other analogous methods due to the small dimensions of the specimen, and several authors mention that it has a lower coefficient of variation (COV) than other methods [6,[11][12][13][14].However, most of these studies work with steel fibers.Therefore, it is important to know the technical and statistical reliability of the Barcelona method as a decision-making tool when choosing the most appropriate method.
Mechanical tests to obtain the post-cracking behavior of FRC are part of the quality control at construction sites.The three-point bending test (3 PB), established in the European Standard EN 14651 [15], specifies a method for determining the flexural tensile strength of concrete with metallic fibers.This method calculates the limit of proportionality (LOP) and residual strength values.The four-point bending test (4 PB), specified in ASTM C1609 [16], evaluates the flexural behavior of FRC using parameters derived from the load-deflection curve obtained by testing a supported beam under loads applied.It lets us know the cracking load, residual strengths, and toughness.However, these tests are characterized by their high dispersion of results because the beams present a small fracture surface [11].
Moreover, the properties depend directly on the specific number of fibers in the cracked section [12].Alternatively, EN 14488 [17] and ASTM C1550 [18] allow calculating the flexural toughness of FRC through square and circular panels subjected to a central point load.The double punch test (DPT) of Molins et al. [19] is an alternative to evaluate the post-cracking behavior of FRC.This "Barcelona method" test presents less dispersion with a COV of results below 13% [20].The standard developed for this test is UNE 83 515 [21].This method allows for determining FRC's cracking resistance, toughness, and residual tensile strength.In addition, it has proven to be suitable for controlling FRC on-site.Unlike the 3 PB and 4 PB flexural tests, the double punching test is characterized by using cylindrical specimens with larger cracking surfaces [22].
In general, it is known that the higher the reinforcement index (RI), the higher the toughness of concrete [23,24].Carmona et al. [25] studied six FRC mixtures with different amounts of steel fibers and plastic fibers to measure the circumferential and axial displacement of the specimens during the tests.The results showed that as the fiber content increases, the results present a higher dispersion in the range of 4.78 to 14.35%.Carmona et al. [12] introduced the concept of toughness index to quantify the post-cracking behavior of FRC with steel fibers, with results showing a dispersion between 5.56 and 14.41%.Aire et al. [26] conducted a comparative study applying the Barcelona test between direct tensile strength and toughness results in 100 × 150 mm molded specimens and 93 × 153 mm control specimens of FRC with steel fibers.The dispersion of their results measured at 4 mm circumferential elongation varied in the range of 13.2 to 35.7%.Molins et al. [19] studied the influence of fiber addition on the toughness of concrete.Their results indicated variability ranges of 13.1 to 22.5%.
Investigations about the post-cracking properties of normal-strength concrete with polypropylene fibers are limited.Del Savio et al. (2023) [27] concluded with a strong correlation between fiber parameters and post-cracking properties with a Pearson's correlation coefficient, r of 0.90.Molins et al. [19] demonstrated a direct correlation between toughness calculated using the Barcelona method and the beam flexural method.Choumanidis [3], using the Barcelona method, found that polypropylene fibers perform better when the crack width is larger than steel fibers.This conclusion was supported by comparing the slopes of the total circumferential opening displacement (TCOD) curve versus toughness for crack widths of 0.5 mm and 3.5 mm, respectively; the percentage dif- ference in slopes increased from 10% to 41% with a larger crack width.Carmona et al. [22] found that more synthetic fibers lead to greater toughness when testing concrete specimens with 4, 8, and 12 kg/m 3 of synthetic fibers.The influence of slenderness and RI on residual strength and toughness of concrete calculated through the Barcelona method has not been reported, and it is important to expand the understanding beyond fiber volume to consider the influence of the RI.In a separate study, Del Savio (2022) [28] investigated the correlation between the RI and the mechanical properties of concrete.This investigation employed two methods: Ultrasonic Pulse Tests (UPV) and dynamic elasticity modulus.Additionally, developing predictive equations for statistically correlated relationships is essential.
The search for a simple, fast method with reliable results is fundamental to establishing adequate quality control of the post-cracking behavior of polypropylene fiber-reinforced concrete (PPFRC).In this study, the post-cracking behavior of FRC, toughness, and residual strength were evaluated through the DPT, also known as the "Barcelona method," by varying polypropylene fiber properties, length (l), volume (V_f), and the RI.Then, a statistical analysis was made to study the correlations of independent variables (IV) with the post-cracking properties, which consisted first of elaborating a total of 10 specimens per concrete mixture, resulting in the testing of 100 specimens.Following this, hypothesis tests were performed to determine each correlation's significance value (p).In addition, the coefficient of toughness variation at different casting locations and with different types of fibers used in the fiber-reinforced concrete was evaluated using previous research results.Finally, a predictive equation was developed to calculate toughness and residual strength as a function of the RI.The experimental plan was developed using three dosages of polypropylene fibers with values corresponding to 0.4, 0.8, and 1.2%.Three fiber lengths were also used: 40, 50, and 60 mm.The test was performed according to the UNE 83515 standard developed in Spain by AENOR [21].This research is organized in the following order: in Section 1, the introduction is presented.Section 2 presents the characteristics of concrete, including aggregate properties, mix design, and experimental procedure.It also includes the definition of the hypothesis test.The execution of the experimental test is described in Section 2. Section 3 presents the discussion and analysis of the results and the formulation of a predictive equation for toughness based on the FRC experimental results.Finally, the conclusions are specified in Section 4.

Research Design
Fiber-reinforced concrete was made with type I Portland cement according to ASTM C150 [29].This cement is characterized by being general purpose, having a high heat of hydration, and rapid strength development.
The coarse aggregate (CA) used was crushed stone.According to their gradation, the coarse aggregates comply with HUSO N • 56 according to ASTM C33 [30].The CA had a maximum nominal size of 25.4 mm.The sand used was river sand and met the particle size requirements of ASTM C33 standard.The fineness modulus of the natural river fine aggregate was 2.95.The particle size curve of the aggregates is shown in Figure 1.
The PP fibers used had a density of 910 kg/m 3 , a modulus of elasticity (E) of 4.70 GPa, and a tensile strength (f_t) of 540 MPa.The length of the fibers was variable, 40, 50, and 60 mm.All fibers had the same diameter of 0.86 mm.
A high-range water-reducing and retarding additive type G, according to ASTM C494 [31], with a density of 1200 kg/m 3 , was used.

Specimen
The concrete was designed to achieve a strength of 40 MPa and a slump of 100 mm.The design method used was the ACI [32].The water-cement ratio was 0.45.The highrange water-reducing admixture was placed at a dosage of 1.40% by weight of the cement.Fibers were placed in three dosages (0.4, 0.8, and 1.2%) and three lengths (40, 50 and 60 mm).The mixed designs are shown in Table 1.

Barcelona Test
The Barcelona method was performed according to the UNE 83515 standard developed in Spain by AENOR [21].The objective of the test was to determine the toughness of the concrete reinforced with fibers, measured in Joules (J).The test was performed on cylindrical specimens with a diameter of 150 mm and a height of 150 mm.The Barcelona method consists of subjecting the FRC to a double punch test employing two cylindrical steel punches, with a height of 24 mm and a diameter of 37.5 mm, centered on the lower and upper surfaces of the specimens.A circumferential extensometer is placed at the midheight of the specimen using a high-precision chain instrument.This instrument allows measurement of the total circumferential opening displacement (TCOD) connected to a clip-gauge.The press piston applies a constant axial displacement rate of 0.5 mm/min.The test ends when the axial displacement is at least 6 mm. Figure 2 shows the laboratory test setup.

Specimen
The concrete was designed to achieve a strength of 40 MPa and a slump of 100 mm.The design method used was the ACI [32].The water-cement ratio was 0.45.The highrange water-reducing admixture was placed at a dosage of 1.40% by weight of the cement.Fibers were placed in three dosages (0.4, 0.8, and 1.2%) and three lengths (40, 50 and 60 mm).The mixed designs are shown in Table 1.

Barcelona Test
The Barcelona method was performed according to the UNE 83515 standard developed in Spain by AENOR [21].The objective of the test was to determine the toughness of the concrete reinforced with fibers, measured in Joules (J).The test was performed on cylindrical specimens with a diameter of 150 mm and a height of 150 mm.The Barcelona method consists of subjecting the FRC to a double punch test employing two cylindrical steel punches, with a height of 24 mm and a diameter of 37.5 mm, centered on the lower and upper surfaces of the specimens.A circumferential extensometer is placed at the midheight of the specimen using a high-precision chain instrument.This instrument allows measurement of the total circumferential opening displacement (TCOD) connected to a clip-gauge.The press piston applies a constant axial displacement rate of 0.5 mm/min.The test ends when the axial displacement is at least 6 mm. Figure 2 shows the laboratory test setup.where P_max (N) is the maximum load that produces cracking, a (mm) is the diameter of the load application disk, and H (mm) is the height of the specimen.Figure 3 represents the curve resulting from the Barcelona test, where P_RX is the residual load for a TCOD of RX mm, P_R6 is the residual load for a TCOD of 6 mm.A total of 10 cylindrical specimens were made for each mixture for further statistical support.The methodology proposed by Gill et al. for rock masses [33] was used to determine this quantity.One of the curves from each series was selected as the representative curve to visualize the shape of at least one of the resulting curves.

Mixing Procedure
The mixing procedure was carried out in four stages.In the first stage, 30% of the total water was added along with 100% of the coarse aggregate and mixed for 30 s.In the second stage, 100% of the fine aggregate was added and mixed again for 30 s.In the third stage, 100% of the cement was added, and 60% of the total water was mixed for 1 min.In this stage, the fibers were added progressively until the mixing was finished.Finally, the remaining water was added with the high-range water-reducing additive and mixed for 5 min.The molds were filled in three equal layers and compacted by rodding for the fresh where P_max (N) is the maximum load that produces cracking, a (mm) is the diameter of the load application disk, and H (mm) is the height of the specimen.Figure 3 represents the curve resulting from the Barcelona test, where P_RX is the residual load for a TCOD of RX mm, P_R6 is the residual load for a TCOD of 6 mm.The indirect tensile strength of the Barcelona test was determined through the formulation proposed by UNE 83515 in Equation (1).
where P_max (N) is the maximum load that produces cracking, a (mm) is the diameter of the load application disk, and H (mm) is the height of the specimen.Figure 3 represents the curve resulting from the Barcelona test, where P_RX is the residual load for a TCOD of RX mm, P_R6 is the residual load for a TCOD of 6 mm.A total of 10 cylindrical specimens were made for each mixture for further statistical support.The methodology proposed by Gill et al. for rock masses [33] was used to determine this quantity.One of the curves from each series was selected as the representative curve to visualize the shape of at least one of the resulting curves.

Mixing Procedure
The mixing procedure was carried out in four stages.In the first stage, 30% of the total water was added along with 100% of the coarse aggregate and mixed for 30 s.In the second stage, 100% of the fine aggregate was added and mixed again for 30 s.In the third stage, 100% of the cement was added, and 60% of the total water was mixed for 1 min.In this stage, the fibers were added progressively until the mixing was finished.Finally, the remaining water was added with the high-range water-reducing additive and mixed for 5 min.The molds were filled in three equal layers and compacted by rodding for the fresh A total of 10 cylindrical specimens were made for each mixture for further statistical support.The methodology proposed by Gill et al. for rock masses [33] was used to determine this quantity.One of the curves from each series was selected as the representative curve to visualize the shape of at least one of the resulting curves.

Mixing Procedure
The mixing procedure was carried out in four stages.In the first stage, 30% of the total water was added along with 100% of the coarse aggregate and mixed for 30 s.In the second stage, 100% of the fine aggregate was added and mixed again for 30 s.In the third stage, 100% of the cement was added, and 60% of the total water was mixed for 1 min.In this stage, the fibers were added progressively until the mixing was finished.Finally, the remaining water was added with the high-range water-reducing additive and mixed for 5 min.The molds were filled in three equal layers and compacted by rodding for the fresh concrete slump tests.For pouring, the 150 mm × 150 mm metallic cylinders were filled with fiber concrete in three layers and compacted manually using a tamping rod.For the slump test and pouring, the layers were compacted 25 times using a tamping rod to ensure uniformity of the concrete.Shortly after that, screeding was performed with a screeding trowel.One day later, the samples were demolded and placed in an outdoor curing pool for 28 days.Figure 4 shows the concrete pouring sequence in metallic cylinders.
, x FOR PEER REVIEW 6 of 17 concrete slump tests.For pouring, the 150 mm × 150 mm metallic cylinders were filled with fiber concrete in three layers and compacted manually using a tamping rod.For the slump test and pouring, the layers were compacted 25 times using a tamping rod to ensure uniformity of the concrete.Shortly after that, screeding was performed with a screeding trowel.One day later, the samples were demolded and placed in an outdoor curing pool for 28 days.Figure 4 shows the concrete pouring sequence in metallic cylinders.

Hypothesis Test
Pearson's hypothesis test is valuable for confirming the statistical significance of correlations between variables.The outcomes of Pearson's test are p-value and R-value, which indicate the significance level and correlation coefficient (R), respectively.Together, these values quantify the correlation's strength between variables.The p-value indicates the probability of being wrong.The significance level is expressed in terms of probability, and the most common values are 0.05 and 0.01 [34].However, in previous studies, it has been found advantageous to set this value as 0.10 for materials exhibiting a high coefficient of variation [10,27,28,35].
Furthermore, the null hypothesis contradicts or denies what the research hypothesis affirms; in essence, it serves as the counterpart to the research hypothesis [34].In this research, the null hypothesis can be rejected or not rejected according to the significance level results.If the p-value is less than 0.10, the null hypothesis is rejected.The null hypothesis is not rejected if the p-value is more than 0.10.
The R-value is the correlation coefficient of the linear regression.R-value between 0% and 5% means that the correlation does not exist; between 5% and 20% is very poor; between 20% and 40% is poor; between 40% and 60% is moderate; between 60% and 80% is considerable; between 80% and 95% is strong; between 95% to 99.9% is very strong; and a value of 100% is perfect.

Results and Analysis
The results of the FRC in fresh and hardened states and their respective COV are presented in Table 2.According to the data obtained from the hardened condition tests, it was found that the average value of compressive (f_c) and tensile strength (f_t) was 42.2 MPa and 5.6 MPa, respectively

Hypothesis Test
Pearson's hypothesis test is valuable for confirming the statistical significance of correlations between variables.The outcomes of Pearson's test are p-value and R-value, which indicate the significance level and correlation coefficient (R), respectively.Together, these values quantify the correlation's strength between variables.The p-value indicates the probability of being wrong.The significance level is expressed in terms of probability, and the most common values are 0.05 and 0.01 [34].However, in previous studies, it has been found advantageous to set this value as 0.10 for materials exhibiting a high coefficient of variation [10,27,28,35].
Furthermore, the null hypothesis contradicts or denies what the research hypothesis affirms; in essence, it serves as the counterpart to the research hypothesis [34].In this research, the null hypothesis can be rejected or not rejected according to the significance level results.If the p-value is less than 0.10, the null hypothesis is rejected.The null hypothesis is not rejected if the p-value is more than 0.10.
The R-value is the correlation coefficient of the linear regression.R-value between 0% and 5% means that the correlation does not exist; between 5% and 20% is very poor; between 20% and 40% is poor; between 40% and 60% is moderate; between 60% and 80% is considerable; between 80% and 95% is strong; between 95% to 99.9% is very strong; and a value of 100% is perfect.

Results and Analysis
The results of the FRC in fresh and hardened states and their respective COV are presented in Table 2.According to the data obtained from the hardened condition tests, it was found that the average value of compressive (f_c) and tensile strength (f_t) was 42.2 MPa and 5.6 MPa, respectively.Figure 5 shows the test's Total Crack Opening Displacement (TCOD) diagram.The gray lines represent the resulting curves, and the blue lines symbolize the representative curves.In Figure 5a, a brittle fracture is observed corresponding to the pattern.In the case of FRC mixtures, they presented a similar behavior after fracture.A significant decrease in strength was noticeable, followed by a softening behavior in the curve.It is important to note that the strength of all mixtures appeared to converge around 140 kN.In Figure 5b, representing the mixture with the lowest RI, the strength initially decreased from 140 kN to 40 kN, corresponding to a 71% reduction in strength.Subsequently, a softening behavior in the curve decreased from 40 kN to 30 kN when 6 mm of elongation was reached.However, in Figure 5j, corresponding to the mixture with the highest RI, the strength decreased from 140 kN to 60 kN initially, representing an approximately 57% reduction.Furthermore, this sample presented a gradual softening behavior that reduced the strength from 60 kN to 40 kN when 6 mm of elongation was reached.Figure 5 shows the test's Total Crack Opening Displacement (TCOD) diagram.The gray lines represent the resulting curves, and the blue lines symbolize the representative curves.In Figure 5a, a brittle fracture is observed corresponding to the pattern.In the case of FRC mixtures, they presented a similar behavior after fracture.A significant decrease in strength was noticeable, followed by a softening behavior in the curve.It is important to note that the strength of all mixtures appeared to converge around 140 kN.In Figure 5b, representing the mixture with the lowest RI, the strength initially decreased from 140 kN to 40 kN, corresponding to a 71% reduction in strength.Subsequently, a softening behavior in the curve decreased from 40 kN to 30 kN when 6 mm of elongation was reached.However, in Figure 5j, corresponding to the mixture with the highest RI, the strength decreased from 140 kN to 60 kN initially, representing an approximately 57% reduction.Furthermore, this sample presented a gradual softening behavior that reduced the strength from 60 kN to 40 kN when 6 mm of elongation was reached.Table 3 shows the flexural mechanical properties of concrete reinforced with polypropylene fibers using the Barcelona test.For elastic properties, the maximum applied load (P_max) and the flexural tensile strength (f_ct) are shown.Regarding post-cracking properties, the results of residual load (P_4 mm, P_6 mm), residual strength (f_res_4 mm, f_res_6 mm), and toughness (T_4 mm, T_6 mm), all measured up to a deflection of 4 and 6 mm, respectively, are shown.The mixture with a 0.8% dosage and 50 mm of fiber length presented a Toughness, at 4 mm of elongation, of 227.1 N×m with a COV of 15.4%.Pujadas et al. [36] achieved a Toughness, at 4 mm, of 265.8 N*m with a COV of 11.6% for a mixture with 0.99% dosage and a fiber length of 48 mm.Molins et al. [19] obtained a toughness of 233.8 N×m with a COV of 22.5% using a dosage of 0.71% and a fiber length of 48 mm.Carmona et al. [22] achieved a toughness of 230.0 N×m with a dosage of 0.88% and a fiber length of 54 mm.Table 3 shows the flexural mechanical properties concrete reinforced with polypropylene fibers using the Barcelona test.For elastic properties, the maximum applied load (P_max) and the flexural tensile strength (f_ct) are shown.Regarding post-cracking properties, the results of residual load (P_4 mm, P_6 mm), residual strength (f_res_4 mm, f_res_6 mm), and toughness (T_4 mm, T_6 mm), all measured up to a deflection of 4 and 6 mm, respectively, are shown.The mixture with a 0.8% dosage and 50 mm of fiber length presented a Toughness, at 4 mm of elongation, of 227.1 N × m with a COV of 15.4%.Pujadas et al. [36] achieved a Toughness, at 4 mm, of 265.8 N × m with a COV of 11.6% for a mixture with 0.99% dosage and a fiber length of 48 mm.Molins et al. [19] obtained a toughness of 233.8 N × m with a COV of 22.5% using a dosage of 0.71% and a fiber length of 48 mm.Carmona et al. [22] achieved a toughness of 230.0 N × m with a dosage of 0.88% and a fiber length of 54 mm.

Post-Cracking Properties
Table 4 shows the results of Pearson's 35 hypothesis tests between the variables of the polypropylene fibers: slenderness (l/d), fiber volume (V_f), and reinforcement index (RI = V_f × l/d), and the post-cracking properties of the concrete: tensile strength, residual strength, and toughness.This analysis concluded that there was no correlation between fiber volume, slenderness, and reinforcement index in the tensile strength calculated using the Barcelona method because the p-value in all correlations, from 1 to 7, was greater than 0.100.The correlations with the residual strength calculated at 4 mm and 6 mm were specified in items 8 to 21.It was observed that there was a correlation between fiber volume and residual strength.However, the slenderness did not influence the residual strengths.There was a correlation with the reinforcement index in f_res_4 mm and f_res_6 mm.The correlations with toughness calculated at 4 mm and 6 mm TCOD are shown in items 22 to 35.The results showed no correlation between the fibers' volume and the calculated toughness.On the other hand, there was a correlation between fiber slenderness and toughness, but only for low fiber volumes, 0.4%.Finally, there was a correlation between the reinforcement index and toughness in both cases, T_4 mm and T_6 mm.

Toughness
Figure 6a shows the trend lines of the relation between toughness and fiber reinforcement index measured for 4 and 6 mm TCOD.The RI is the product of slenderness and fiber volume.The p-values of the correlation between toughness and RI for tests performed up to 4 and 6 mm strain were 0.039 and 0.044, respectively.It was observed that these correlations were significant since both values were less than 0.100.The correlation coefficients, R, were 0.69 and 0.68, respectively, indicating considerable correlations.Finally, the trend line showed that an increase of 10 RI units will increase 12.98 J for T_6 mm and 8.86 J for T_4 mm. Figure 6b shows the relation between the coefficient of toughness variation with the strengthening index.From the analysis, the higher the RI, the lower the COV.This is supported by Pearson's test, which resulted in a p-value of 0.041, rejecting the null hypothesis.

Toughness
Figure 6a shows the trend lines of the relation between toughness and fiber reinforcement index measured for 4 and 6 mm TCOD.The RI is the product of slenderness and fiber volume.The p-values of the correlation between toughness and RI for tests performed up to 4 and 6 mm strain were 0.039 and 0.044, respectively.It was observed that these correlations were significant since both values were less than 0.100.The correlation coefficients, R, were 0.69 and 0.68, respectively, indicating considerable correlations.Finally, the trend line showed that an increase of 10 RI units will increase 12.98 J for T_6 mm and 8.86 J for T_4 mm. Figure 6b shows the relation between the coefficient of toughness variation with the strengthening index.From the analysis, the higher the RI, the lower the COV.This is supported by Pearson's test, which resulted in a p-value of 0.041, rejecting the null hypothesis.From the linear regressions of T_6 mm and T_4 mm with the RI, Equations (2) and (3), valid for synthetic fibers, are obtained: These equations are useful to calculate the toughness as a function of the reinforcement index of polypropylene fibers for concrete with compressive strengths of 40 to 45 MPa, Figure 8 shows that the increase in residual strength due to the increase in fiber volume was independent of the fiber slenderness used, with an average value of 1.88 MPa for f_res_4 mm and 1.47 for f_res_6 mm.Finally, the maximum residual strength corresponding to f_res_4 mm was that of the D:1.2-50 blend with a value of 2.49 MPa; similarly, for f_res_6 mm, the maximum residual strength was that of the D:1.2-50 blend with a value of 1.9 MPa. Figure 8 shows that the increase in residual strength due to the increase in fiber volume was independent of the fiber slenderness used, with an average value of 1.88 MPa for f_res_4 mm and 1.47 for f_res_6 mm.Finally, the maximum residual strength corresponding to f_res_4 mm was that of the D:1.2-50 blend with a value of 2.49 MPa; similarly, for f_res_6 mm, the maximum residual strength was that of the D:1.2-50 blend with a value of 1.9 MPa.
These equations are useful to calculate the toughness as a function of the reinforcement index of polypropylene fibers for concrete with compressive strengths of 40 to 45 MPa, slump ranging from 46 to 240 mm, made with aggregates with a maximum nominal size of 25.4 mm.

Residual Strength
Linear regression allows predicting the behavior of the residual strength measured at TCOD of 4 and 6 mm from the dosage values in the fibers' volume.Figure 7 shows the lines representing the trend of residual strength concerning fiber volume.For the residual strengths measured at 4 mm, the p-values of the correlations were 0.083, 0.071, and 0.117 for slenderness of 47, 58, and 70, respectively.For the residual strengths measured at 6 mm, the p-values were 0.077, 0.071, and 0.035, respectively.These correlations were statistically significant since five of the six values were less than 0.100.Consequently, the hypothesis that there is a correlation between variables was accepted.Figure 8 shows that the increase in residual strength due to the increase in fiber volume was independent of the fiber slenderness used, with an average value of 1.88 MPa for f_res_4 mm and 1.47 for f_res_6 mm.Finally, the maximum residual strength corresponding to f_res_4 mm was that of the D:1.2-50 blend with a value of 2.49 MPa; similarly, for f_res_6 mm, the maximum residual strength was that of the D:1.2-50 blend with a value of 1.9 MPa. Figure 9 shows the relation between the residual strength of concrete and the fiber RI for 4 and 6 mm TCOD.The p-values for the correlations between residual strength and RI were 0.006 and 0.002.These figures are very close to zero.Therefore, the probability of error was low.The correlation coefficients, R, were 0.82 and 0.85 for the 4 and 6 mm TCOD, respectively.This shows strong correlations in both cases.Finally, the trend line shows that 10 RI units will increase by 0.124 for f_res_6 mm and 0.137 MPa for f_res_4 mm. Figure 9 shows the relation between the residual strength of concrete and the fiber RI for 4 and 6 mm TCOD.The p-values for the correlations between residual strength and RI were 0.006 and 0.002.These figures are very close to zero.Therefore, the probability of error was low.The correlation coefficients, R, were 0.82 and 0.85 for the 4 and 6 mm TCOD, respectively.This shows strong correlations in both cases.Finally, the trend line shows that 10 RI units will increase by 0.124 for f_res_6 mm and 0.137 MPa for f_res_4 mm.
These equations are useful, as in toughness, to calculate the residual strength as a function of the RI of polypropylene fibers for concrete with compressive strength of 40 to 45 MPa, slump ranging from 46 to 240 mm, elaborated with aggregates with a maximum nominal size of 25.4 mm.
Figure 10 shows graphically the existence of a correlation between the variables studied.In general, it can be concluded that flexural strength is not determined by the placement of fibers in the mix; rather, it is determined by the concrete matrix.The residual strengths are influenced by the volume of fibers and by the RI.It may seem that the latter is a consequence of the former.Still, the significance level of the correlations with the RI was lower than in the case of the correlations with the volume of fibers.In other words, although the hypothesis that there is no correlation between fiber slenderness and residual strength cannot be rejected, slenderness does have an influence, although to a lesser degree.Finally, toughness was not influenced by fiber volume or slenderness when these were modified separately; but it was influenced by the combined effect of both, i.e., by the RI.These equations are useful, as in toughness, to calculate the residual strength as a function of the RI of polypropylene fibers for concrete with compressive strength of 40 to 45 MPa, slump ranging from 46 to 240 mm, elaborated with aggregates with a maximum nominal size of 25.4 mm.
Figure 10 shows graphically the existence of a correlation between the variables studied.In general, it can be concluded that flexural strength is not determined by the placement of fibers in the mix; rather, it is determined by the concrete matrix.The residual strengths are influenced by the volume of fibers and by the RI.It may seem that the latter is a consequence of the former.Still, the significance level of the correlations with the RI was lower than in the case of the correlations with the volume of fibers.In other words, although the hypothesis that there is no correlation between fiber slenderness and residual strength cannot be rejected, slenderness does have an influence, although to a lesser degree.Finally, toughness was not influenced by fiber volume or slenderness when these were modified separately; but it was influenced by the combined effect of both, i.e., by the RI.

Comparative Analysis of Toughness as a Function of RI
A compilation of results of toughness and residual strength calculated using the Barcelona method was made (see Table 5).The most studied fibers were steel and synthetic fibers.In addition, the place where the concrete was poured, in the laboratory and the underground mining, was also identified.The modulus of elasticity of the fibers (E), volume ( V_f), length, diameter, slenderness (l/d), and reinforcement index (RI) were identified.In addition, the residual strength and toughness with their respective coefficients of variation were annotated.In Figure 11, one can observe the normalized toughness graph versus the RI.The developed empirical predictive Equations (2) and (3) were applied to the results of other authors collected in Table 5.In all cases, the results are underestimated.For Choumanidis et al.'s results [3], the values were underestimated by 11% compared to the experimental ones; for Molins' results [19], by 20%; whereas for Carmona et al.'s results [22], by 6%.

Figure 6 .
Figure 6.(a) FRC toughness as a function of RI, (b) coefficient of toughness variation as a function of RI.

Figure 6 .
Figure 6.(a) FRC toughness as a function of RI, (b) coefficient of toughness variation as a function of RI.From the linear regressions of T_6 mm and T_4 mm with the RI, Equations (2) and (3), valid for synthetic fibers, are obtained: T_6 mm = 1.298 × RI + 192.91(2)

Figure 7 .
Figure 7. Residual strength as a function of fiber volume.

Figure 8 .Figure 7 .
Figure 8. Increase in toughness per fiber volume as a function of fiber slenderness.

Figure 7 .
Figure 7. Residual strength as a function of fiber volume.

Figure 8 .Figure 8 .
Figure 8. Increase in toughness per fiber volume as a function of fiber slenderness.

Table 2 .
Characteristics of FRC in the fresh and hardened condition.

Table 2 .
Characteristics of FRC in the fresh and hardened condition.

Table 3 .
Flexural mechanical properties of concrete reinforced with polypropylene fibers using the Barcelona test.

Table 4 .
Pearson's hypothesis for correlations between flexural properties and fiber variables.